advertisement

RAPID COMMUNICATIONS PHYSICAL REVIEW B 70, 220102(R) (2004) Properties of Pb„Zr, Ti…O3 ultrathin films under stress-free and open-circuit electrical boundary conditions Emad Almahmoud, Yulia Navtsenya, Igor Kornev, Huaxiang Fu, and L. Bellaiche Physics Department, University of Arkansas, Fayetteville, Arkansas 72701, USA (Received 3 September 2004; published 17 December 2004) A first-principles-based scheme is developed to simulate properties of (001) PbO-terminated Pb共Zr1−xTix兲O3 thin films that are under stress-free and open-circuit boundary conditions. Their low-temperature spontaneous polarization never vanishes down to the minimal thickness, and continuously rotates between the in-plane 具010典 and 具110典 directions when varying the Ti composition around x = 0.50. Such rotation dramatically enhances piezoelectricity and dielectricity. Furthermore, the order of some phase transitions changes when going from bulk to thin films. DOI: 10.1103/PhysRevB.70.220102 PACS number(s): 77.55.⫹f, 77.80.Bh, 77.65.Bn, 77.22.Ch Ferroelectric thin films are currently of enormous technological interest, mostly because of the need for miniaturization in devices.1 Many fundamental questions are still unanswered and/or unsettled in these low-dimensional systems. For instance, whether or not there is a critical thickness below which no ferroelectricity can occur is still under debate.2–6 Similarly, the precise effects of surface on properties of thin films are opened for discussion.5,7–10 One may also wonder how the striking features exhibited by some bulk materials may evolve in the corresponding thin films. Typical examples of such features are the unusual lowsymmetry phases (associated with a composition-induced rotation of the spontaneous polarization and with an enhancement of dielectric and piezoelectric responses), recently discovered in the morphotropic phase boundary (MPB) of various alloys.11–15 One reason behind this lack of knowledge is that thin (and particularly ultrathin) films are difficult to synthesize in a good quality form, and their characterization is by no means straightforward. Similarly, realistically simulating thin films is a theoretical challenge. For instance, while phenomenological and ab initio-based models have already provided a deep insight into thin films (see Refs. 2 and 16–18 and references therein), such models do not usually incorporate some subtle surface-related phenomena, e.g., charge transfer and modification of ferroelectric interactions near the surface. On the other hand, direct first-principles techniques can easily include such effects.3,7–10 However, their large computational cost currently prevents them from being used to study complex phenomena and/or complex systems (e.g., thin films made of disordered solid solutions), especially at finite temperature. The atomistic approach of Ref. 5 is a promising technique for investigating thin films at finite temperature, but its level of accuracy depends on the surface termination,5 which emphasizes that mimicking well surface effects on physical properties is tricky. The aims of this Rapid Communication are twofold: first, to present a first-principles-derived approach allowing accurate predictions of finite-temperature properties of complex ferroelectric thin films, under stress-free and open-circuit boundary conditions; second, to use this approach to better understand thin films by providing answers to the questions mentioned above. 1098-0121/2004/70(22)/220102(4)/$22.50 Here, we extend the ab initio effective Hamiltonian scheme proposed in Ref. 12 to mimic thin films that (1) are made of Pb共Zr, Ti兲O3 (PZT); (2) are grown on a substrate along the [001] direction; and (3) have vacuum above them. More precisely, the total energy Etot of such low-dimensional systems is written as Etot共兵u共i兲其,兵v共i兲其, ,兵i其兲 = Emat共兵u共i兲其,兵v共i兲其, ,兵i其兲 + P +S 兺j uz共j兲 + T 兺j vz共j兲 u␣共j兲关u␣共j + ␣ˆ 兲 + u␣共j − ␣ˆ 兲兴, 兺j ␣兺 =x,y 共1兲 where u共i兲 are the (B-centered) local soft modes in unit cells i of the film, and are directly proportional to the electrical polarization. v共i兲 are inhomogeneous strains around the i site, while is the homogeneous strain tensor. 兵i其 characterizes the alloy configuration.12 Emat represents the intrinsic ferroelectric and elastic interactions inside the film, with its analytical expression and first-principles-derived parameters being those of PZT bulks.12 Only four (out of 26) parameters are composition dependent in Emat: they are those associated with the so-called local-mode self-energy.12 The last three terms of Eq. (1) mimic explicit interactions between this film and the vacuum, with the j index running over all the B sites that are the closest to the free surface. ux共j兲, uy共j兲, and uz共j兲 denote the (x, y and z) Cartesian component of u共j兲 along the pseudocubic [100], [010], and [001] directions, respectively. ␣ runs over the x and y axes (i.e., it does not include the growth direction). u␣共j + ␣ˆ 兲 [respectively, u␣共j − ␣ˆ 兲] is the ␣ component of the local mode centered on the B site that is the closest from the j site that is parallel (respectively, antiparallel) to the ␣ axis. The P and T parameters quantify how vacuum affects the out-of-plane components (uz and vz) of the local modes and inhomogeneous strains near the surface, respectively. S characterizes the change, with respect to the bulk, of the short-range interaction between the in-plane components of the local modes near the surface. The P, T, and S parameters are determined from first-principles calculations on a PbO-terminated (001) 17-atom slab (corresponding to 3 B - O and 4 A - O atomic layers) of a PZT alloy, as 220102-1 ©2004 The American Physical Society RAPID COMMUNICATIONS PHYSICAL REVIEW B 70, 220102(R) (2004) ALMAHMOUD et al. mimicked by the virtual crystal alloy approximation,19 surrounded by a vacuum region being two lattice constants thick.20 Using Eq. (1) with these parameters results in an excellent agreement with first-principles predictions for the layer-by-layer profile of the polarization in various PbOterminated slabs (e.g., in slabs that are not used in the fitting procedure).21 Furthermore, the substrate is assumed to be inert, i.e., no term analogous to the last three expressions of Eq. (1) is considered at the substrate/film interface. The local modes and inhomogeneous strain-related variables are also forced to vanish in the substrate (as well as, of course, in the vacuum), being consistent with the fact that some commonly used substrates (e.g., MgO) are ferroelectric inactive. As a result, dipole-dipole interactions only occur in the film, which automatically guarantees the generation of a depolarizing field inside the film if this latter has a component of its electrical polarization along the growth direction. Our films are thus under open-circuit electrical boundary conditions. Technically, we use the total energy of Eq. (1) in Monte Carlo simulations to compute the finite-temperature properties of PbO-terminated PZT ultrathin films having a number of layers (to be denoted by d) ranging between 1 and 6. These simulations use the Metropolis algorithm,22 and provide the thermodynamically equilibrated local soft modes and strains as outputs for each temperature. The strains (like the local modes, but unlike the alloy configuration that is kept frozen) are allowed to fully relax. Our studied films are thus stress free in terms of mechanical boundary conditions. Typically, we use a huge number of Monte Carlo sweeps (up to 20 million) and large 10⫻ 10⫻ 40 periodic supercells (the regions made of substrate and vacuum are thus altogether 40 − d lattice constants thick along the growth direction) to get well-converged results. The B atoms are randomly distributed in the film. Figure 1 displays the predicted Cartesian coordinates (具ux典, 具uy典, and 具uz典) of the average of the local mode vectors in the ⯝20-Å-thick 共d = 5兲 PZT film having a 50% Ti composition, as a function of the rescaled temperature.23 Two sets of calculations are reported: one incorporating all the surface-related terms of Eq. (1) versus another for which the P, T, and S coefficients are all turned off. In both cases, each coordinate is close to zero at high temperature, indicating a paraelectric phase. As the temperature is cooled down and passes through a Tc critical temperature, 具uy典 jumps and then increases when the temperature further decreases, while 具ux典 and 具uz典 remain nearly null.25 This characterizes a transition to a ferroelectric phase having a polarization pointing along a 具100典 direction, as in the PZT bulk having the same Ti composition of 50%.12 However, the polarization direction in the film can be along either the y axis (as in Fig. 1) or the x axis, but (unlike in the bulk) never along the [001] growth direction (z axis), in order to avoid the generation of a huge depolarizing field.5 Interestingly, we also found (not shown here) that thinner PbO-terminated films, down to d = 1, also exhibit a nonzero in-plane polarization in their ground state. Our calculations thus predict that stress-free PZT films, under open-circuit electrical boundary conditions and with Ti compositions around 50%, do not have any critical thickness FIG. 1. Film average of the cartesian coordinates (具ux典, 具uy典, and 具uz典) of the local modes in the ⯝20-Å-thick 共d = 5兲 PZT film having a 50% Ti composition, as a function of the rescaled temperature. The filled symbols represent predictions when all the surfacerelated parameters of Eq. (1) are turned on, while the open symbols show the corresponding results when neglecting the P, T, and S parameters. The y component of the local modes is indicated via circles, while the triangles and squares display the x and z components, respectively, of these local modes. (The z component of the local modes is always null for each temperature and is not shown for clarity, when neglecting the P, T, and S parameters.) below which ferroelectricity disappears. Such a conclusion seems to contradict recent studies (see, e.g., Ref. 3). However, one has to realize that, e.g., Ref. 3 defines the critical thickness with respect to the vanishing of the component of the polarization along the z axis (while we define it here with respect to the vanishing of all the components of the polarization) and studies thin films that are under a compressive strain and close (but not equal to) short-circuit electrical boundary conditions. The specificity of our present study does not allow us to generalize our findings for the mechanical and electrical boundary conditions associated with some of these previous studies. Figure 1 further tells us that the Tc Curie temperature of the d = 5 PZT film is around 525 K, that is lower by ⯝120 K from the one of the corresponding PZT bulk,24 when turning on P, T, and S in Eq (1). Neglecting such parameters leads to a much smaller Tc共⯝370 K兲. Such a large difference in Tc is found to be mostly due to the S parameter (which characterizes the vacuum-induced change of short-range interaction near the surface). Interestingly, this S parameter is rather sensitive to the surface termination.7 This implies that properties of ultrathin films having two differently terminated surfaces can dramatically differ, even if those films are made from the same material and have similar thickness. Figure 2 sheds more light on surface effects by displaying the layer-by-layer profiles of the local modes for the d = 5 ultrathin film having a Ti composition of 50%, when turning on and off the P, T, and S parameters at 10 K. One can clearly see that, in both cases, the y component of the local dipoles centered in the B layers, which are neither located near the interface nor the surface, has a more or less layerindependent value that is slightly smaller than the one in the bulk 共⯝0.107 a.u.兲. On the other hand, the B layer that is the closest to the substrate/film interface has much smaller inplane dipoles. The P, S, and T parameters also have a sig- 220102-2 RAPID COMMUNICATIONS PHYSICAL REVIEW B 70, 220102(R) (2004) PROPERTIES OF Pb共Zr, Ti兲O3 ULTRATHIN FILMS… FIG. 2. Local modes for the d = 5 PZT ultrathin film as a function of the layer index along the growth direction, at 10 K. An index of 1 characterizes the B layer that is closest to the substrate, while the B layer located near the vacuum has an index of 5. The solid line and filled symbols represent predictions when all the surfacerelated parameters of Eq. (1) are turned on, while the dashed line and open symbols show the corresponding results when neglecting the P, T, and S parameters. The y component of the local modes is indicated via circles, while the squares display the z component of these local modes. (The x component of the local modes is always null in each layer, and is not shown for clarity.) The simulated film has a composition of 50% of Ti. nificant effect on the y component of the dipole in the B layer located near the vacuum: neglecting these parameters generates a small value that is comparable to the one near the interface, while turning them on yields a large enhancement of this y component in this PbO-terminated ultrathin film. Such enhancement is due to the S coefficient, and explains why the Curie temperature of the film increases when turning on the surface-related parameters, since it is commonly accepted that the larger the spontaneous polarization is at small temperature (see Fig. 2) the higher Tc (see Fig. 1).26 Another difference worth noticing between the two kinds of calculations is about the z component of the dipole in the B layer located near the vacuum: the fitted value of the P parameter leads to a uz that does not vanish anymore and that is negative, mostly characterizing Pb displacements oriented inwards the film near the PbO-terminated surface, as consistent with Ref. 8. We now use our scheme to investigate properties of Pb共Zr1−xTix兲O3 films, with a fixed thickness 共d = 5兲 at 10 K, as a function of Ti composition, with all the surface relaxations of Eq. (1) being included. Figure 3(a) shows that the spontaneous polarization is nearly parallel to a 具010典 direction, that is, perpendicular to the growth direction, for Ti compositions larger than 49.6%.25 The associated phase, to be denoted by T, can be considered to be tetragonal when solely focusing on the film (otherwise, it is orthorhombic when including the substrate and vacuum in addition to the film). This polarization becomes nearly parallel to a 具110典 pseudocubic direction25 (i.e., it changes of in-plane direction) for x smaller than 47.0%. This yields a phase that can be classified as orthorhombic and will be denoted as O. One striking feature of Fig. 3(a) is the behavior of the local mode for compositions decreasing between 49.6% and 47.0%: 具uy典 decreases, while 具ux典 smoothly increases, and 具uz典 remains FIG. 3. Properties of the d = 5 ultrathin PZT films as a function of Ti composition, at 10 K. Panel (a) displays the film average of the cartesian coordinates (具ux典, 具uy典 and 具uz典) of the local modes. Panel (b) shows the d22 and d16 piezoelectric coefficients. Panel (c) displays the 11 and 22 dielectric susceptibilities. All the parameters of Eq. (1) are turned on in these simulations. All the calculations are performed using 10⫻ 10⫻ 40 supercells, except those corresponding to a Ti composition around 0.47, for which 20⫻ 20 ⫻ 40 supercells are used to confirm that some piezoelectric and dielectric coefficients peak around this composition, as expected by phase-transition theory. nearly null.25 This characterizes a continuous (in-plane) rotation of the polarization within a (001) plane from a 具010典 to a 具110典 direction, with the resulting phase adopting a monoclinic M C symmetry.27 Interestingly, the phase diagram depicted in Fig. 3(a) can be rather well qualitatively and quantitatively deduced from the one occurring in the MPB of PZT bulks, when imposing the additional constraint that 具uz典 = 0 to these latters. As a matter of fact, at small temperature, the polarization of PZT bulks rotates from a 具010典 (tetragonalassociated) to the 具111典 (rhombohedral-associated) direction, via a recently discovered monoclinic M A phase (characterized by a polarization lying along 具uvu典 with u ⬍ v,11) for Ti compositions decreasing between 49.5 and 47.0%.12 One noticeable difference exists, however, for the nature of the composition-induced phase transition around 47.0% between the bulks and the films: the rhombohedral R-to-monoclinic M A phase transition occurring in the bulk is of first order,12,27 while the orthorhombic O-to-monoclinic M C transition appears to be of second order in the film [see the continuous rotation of the mode in Fig. 3(a)]. Interestingly, such differ- 220102-3 RAPID COMMUNICATIONS PHYSICAL REVIEW B 70, 220102(R) (2004) ALMAHMOUD et al. ence is consistent with the sixth-order Devonshire theory for the R-to-M A and O-to-M C transitions.27 Figures 3(b) and 3(c) reveal that, when representing the dielectric and piezoelectric tensors in the basis formed by the x, y and z axes, the d16 piezoelectric and 11 dielectric coefficients of PZT films not only peak at both transitions (as consistent with phase-transition theory) but also adopt remarkably large values anywhere between 47.0 and 49.5%. As in bulks,12,13,15 these large values result from the composition-induced rotation of the polarization. PZT ultrathin films may thus be promising to design miniaturized ferroelectric devices with large dielectric and piezoelectric responses. In summary, we developed a first-principles-based scheme to investigate finite-temperature properties of (001) PZT stress-free ultrathin films under open-circuit electrical boundary conditions, that are PbO terminated and have a Ti F. Scott, Ferroelectric Memories (Springer, Berlin, 2000). Ghosez and K. M. Rabe, Appl. Phys. Lett. 76, 2767 (2000). 3 J. Junquera and P. Ghosez, Nature (London) 422, 506 (2003). 4 T. Tybell, C. H. Ahn, and J.-M. Triscone, Appl. Phys. Lett. 75, 856 (1999). 5 S. Tinte and M. G. Stachiotti, Phys. Rev. B 64, 235403 (2001). 6 H. Fu and L. Bellaiche, Phys. Rev. Lett. 91, 257601 (2003). 7 B. Meyer and D. Vanderbilt, Phys. Rev. B 63, 205426 (2001). 8 B. Meyer, J. Padilla, and D. Vanderbilt, Faraday Discussions 114: The Surface Science of Metal Oxides (Royal Society of Chemistry, London, 2000), p. 395. 9 R. E. Cohen, J. Phys. Chem. 57, 1393 (1996); Ferroelectrics 194, 323 (1997). 10 L. Fu, E. Yaschenko, L. Resca, and R. Resta, Phys. Rev. B 60, 2697 (1999). 11 B. Noheda, D. E. Cox, G. Shirane, J. A. Gonzalo, L. E. Cross, and S.-E. Park, Appl. Phys. Lett. 74, 2059 (1999). 12 L. Bellaiche, A. García, and D. Vanderbilt, Phys. Rev. Lett. 84, 5427 (2000); Ferroelectrics 266, 41 (2002). 13 H. Fu and R. E. Cohen, Nature (London) 403, 281 (2000). 14 I. Grinberg, V. R. Cooper, and A. M. Rappe, Nature (London) 419, 909 (2002). 15 Z. Wu and H. Krakauer, Phys. Rev. B 68, 014112 (2003). 16 I. Kornev, H. Fu, and L. Bellaiche, Phys. Rev. Lett. 93, 196104 (2004). 17 O. Dieguez, S. Tinte, A. Antons, C. Bungaro, J. B. Neaton, K. M. 1 J. 2 P. composition around 50%. We found that (1) such films do not have any critical thickness below which ferroelectricity disappears; (2) their polarizations are perpendicular to the growth direction; (3) surface effects, and especially vacuuminduced changes of short-range interactions, significantly affect their local and macroscopic properties; (4) these ultrathin films exhibit a morphotropic phase boundary where their polarization continuously rotates, in a (001) plane between a 具010典 and 具110典 direction, as the Ti composition decreases; (5) such rotation leads to large piezoelectricity and dielectricity; and (6) the nature of phase transitions can change when going from bulks to ultrathin films. We thank I. Naumov for useful discussions. This work is supported by ONR Grants No. 00014-01-1-0365, N0001404-1-0413, and 00014-01-1-0600, and by NSF Grants No. DMR-0404335 and DMR-9983678. Rabe, and D. Vanderbilt, Phys. Rev. B 69, 212101 (2004). L. Li, S. Y. Hu, Z. K. Liu, and L. Q. Chen, Appl. Phys. Lett. 81, 427 (2002). 19 L. Bellaiche and D. Vanderbilt, Phys. Rev. B 61, 7877 (2000). 20 We obtained P = + 0.0144, T = + 0.00693, and S = −0.00405 in atomic units. These values were numerically found to be independent on the lateral size, as well as on the number of vacuum layers, of the supercells used within the approach of Eq. (1) to fit the first-principles calculations on the 17-atom slab. We also assume that these parameters are composition-independent since none of them is associated with the local-mode self-energy [which is the energy that is rather sensitive to concentration in PZT bulks (Ref. 12)]. 21 Note that Ref. 8 predicts that the PbO-terminated surface is the most stable one in PbTiO3-like compounds. 22 N. Metropolis, A. Rosenbluth, M. Rosenbluth, M. Teller, and E. Teller, J. Chem. Phys. 21, 1087 (1953). 23 As in Ref. 12 and some references therein, our temperatures are rescaled down by a constant factor so that the theoretical Curie temperature in disordered Pb共Zr0.5xTi0.5兲O3 bulk is forced to match the experimental value of 642 K (Ref. 24). 24 T. Yamamoto, Jpn. J. Appl. Phys., Part 1 35, 5104 (1996). 25 Note that, in fact, 具u 典 is slightly negative, when all the paramz eters of Eq. (1) are turned on. For the sake of simplicity, we neglect such small value in the discussion. 26 A. D. Bruce, Adv. Phys. 29, 111 (1980). 27 D. Vanderbilt and M. H. Cohen, Phys. Rev. B 63, 094108 (2001). 18 Y. 220102-4